inspection & sampling procedures for fine & coarse aggregates
Post on 30-Dec-2016
Embed Size (px)
Inspection & Sampling Procedures for Fine & Coarse
TABLE OF CONTENTS
CHAPTER ONE - TESTING EQUIPMENT
Deleterious and Chert
Test Equipment Verification
CHAPTER TWO - SAMPLING
Size of Original Samples
Method of Sampling
Sampling Directly from Trucks, Rail Cars, or Barges
CHAPTER THREE - SAMPLE REDUCTION
Reducing a Sample to Test Size
Size of Test Sample (After Splitting)
CHAPTER FOUR - TESTING
Sieve Analysis Test
Sieve Analysis for Dense Gradation materials
Deleterious Materials in Coarse Materials
Deleterious Materials in Natural Sand
Flat and Elongated Particles
Fine Aggregate Angularity
Surface Moisture Tests
CHAPTER FIVE - AGGREGATE SPECIFICATIONS AND REQUIREMENTS
Physical Quality Requirements
Physical Quality Tests
General Usage Requirements
B Borrow and Structure Backfill
Aggregate Pavements or Shoulders
Summary of Gradation Requirements
Indiana Test Methods
202 Acid Insoluble Content of Fine Aggregates
203 Control Procedures for Classification of Aggregates
205 Acceptance Procedures for Dolomite Aggregates
206 Scratch Hardness of Coarse Aggregate Particles
207 Sampling Stockpiled Aggregates
209 Soundness of Aggregates by Freezing and Thawing in a Brine
210 Class AP Coarse Aggregate for Concrete Pavement and Slab-on-
212 Acceptance Procedures of Air Cooled Blast Furnace Slag for
902 Verifying Sieves
903 Verifying Ovens
906 Verifying Mechanical Shakers
910 Verifying Balances
AASHTO Test Methods
T 2 Sampling of Aggregates
T 11 Materials Finer Than 75 m (No. 200) Sieve in Mineral
Aggregates by Washing
T 27 Sieve Analysis of Fine and Coarse Aggregates
T 84 Specific Gravity and Absorption of Fine Aggregate
T 85 Specific Gravity and Absorption of Coarse Aggregate
T 112 Clay Lumps and Friable Particles in Aggregate
T 248 Reducing Field Samples of Aggregate to Testing Size
T 304 Uncompacted Void Content of Fine Aggregate
ASTM Test Methods
D 4791 Flat Particles, Elongated Particles, or Flat and Elongated
Particles in Coarse Aggregate
D 5821 Determining Percent of Fractured Particles in Coarse
1 Testing Equipment
Deleterious and Chert
Test Equipment Verification
1 CHAPTER ONE:
The following equipment and supplies are deemed necessary to properly
perform the various required tests for aggregate inspection. The technician
will have on hand, or have access to sufficient quantities of these supplies
or equipment before attempting to conduct tests.
Equipment required for various general procedures:
1) Electronic balance, Class G2, general purpose balance in accordance with AASHTO M 231. The balance shall be readable to 0.1 g and
accurate to 0.2 g or 0.1% of the test load, whichever is greater,
throughout the range of use.
2) Laboratory oven capable of maintaining a temperature of 230 9 F,. (gas burners or electric hot plates may be used).
3) Metal pans for drying and storage
4) Utensils for washing and drying samples, such as trowels, spatulas, etc.
5) Appropriate data sheets, log books, etc.
Equipment required for AASHTO T 2 or ITM 207:
1) Square-nose shovel
2) Sample tube for sand
3) Containers, such as 20 gallon buckets, plastic fiber bag, etc. Galvanized bushel tubs work well.
4) Labels of sufficient size to allow for proper identification of samples.
5) Templates for belt sampling.
Equipment required for AASHTO T 248:
1) Mechanical splitters
Equipment required for AASHTO T 27
1) Sieves - for coarse aggregates 15 in. x 23 in. or 14 in. x 14 in. screens are recommended with sieve designations 2 in., 1 1/2 in., 1 in., 3/4 in.,
1/2 in., 3/8 in., No. 4, No.8 and pan. For fine aggregates 8 in. round
sieves are standard with sieve designations 3/8 in., No. 4, No. 8, No. 16,
No. 30, No. 50, No. 100, No. 200, and pan.
2) Mechanical sieve shaker -- appropriate model to accommodate sieves.
3) Sieve brushes -- Wire and bristle brushes (a wire brush will damage a No. 50 or smaller sieve).
Equipment required for AASHTO T 11:
1) Sieves - No. 16 and No. 200. The No. 200 sieve can be protected from punctures and tears by covering with a No. 16 sieve.
2) Container - size sufficient to contain the sample covered with water and permit vigorous agitation.
3) Wetting Agent - such as liquid detergent, etc. Some fine materials, especially limestone dust, require a wetting agent to break the surface
tension of the particles. A drop or 2 of dish washing liquid is usually
4) Decant Machine - may be used provided the results are consistent with those obtained using manual operations.
Deleterious and Chert
1) Scratch hardness tester.
2) Hydrochloric acid and glass plate.
TEST EQUIPMENT VERIFICATION
The test equipment shall be properly verified, and maintained within the
limits described in the applicable test method. The Certified Aggregate
Producer Program requires equipment to be verified prior to beginning
testing in the Coordinated Testing Phase and also at a minimum frequency
EQUIPMENT REQUIREMENT MINIMUM
Balances Verification 12 mo. ITM 910
thoroughness 12 mo. ITM 906
Sieves Check physical
thoroughness 12 mo. ITM 902
Proper organization of the laboratory is necessary in order to maximize
efficiency and minimize problems and erroneous results. Special
consideration should be given to the flow of the work to be done and the
laboratory organized in the direction of this flow. For example, one might
arrange the equipment from left to right when running sieve analyses as
1) Riffle splitter -- for reduction of incoming samples.
2) Oven -- for drying samples after reduction.
3) Cooling rack and fan -- for cooling samples when dry (note: make sure that the fan does not blow towards the balance in the weighing area and
does not disperse sample fines).
4) Coarse aggregate shaker.
5) Fine aggregate shaker.
6) Weighing area -- balance should be in an area free from vibration, dust, and air flow.
Every laboratory situation is different. The lab should be set up to meet
the flow requirements of the most routine test performed. The need for
back-tracking should be minimized, especially if more than one technician
is working at a time. A little extra time and thought to the set up of the lab
will significantly increase productivity and decrease turn-around time.
Sampling Techniques Safety Sample References Size of Original Samples Sample Type Method of Sampling Production Sampling Stockpile Sampling Sampling Directly from Trucks, Rail Cars, or Barges
2 CHAPTER TWO: SAMPLING
Sampling is perhaps the most important step in assuring that good quality aggregates are being used. Since a sample is just a small portion of the total material, the importance that the sample be representative of the material being delivered can not be overemphasized. Any test performed on the sample, regardless of how carefully and accurately performed, is worthless unless the sample is truly representative of the material offered for use on the project.
The sampling of materials can expose the technician to machinery, moving belts, large stockpiles, and other potential dangers. Proper safety practices are always the first concern. When not sure of safety the technician should stop and seek the supervisors instructions.
A representative sample can be obtained